The University of North Carolina LIBRARY
COLLEGE COLLECTIONGift of oly
EFFECT OK SELECTED FABRIC SOFTENERS ON THE SURFACE APPEARANCE AND PHYSICAL PROPERTIES OF
COTTON WASH-WEAR FABRICS
Mary Regina Neely
A Thesis Submitted to
the Faculty of the Graduate School at
The Woman's College of the University of North Carolina in Partial Fulfillment
of the Requirements for the Degree I.iaster of Science in Hone Economics
Greensboro November, 1962
This thesis has been approved by the following committee of the Faculty of the Graduate School at the Woman's College of the University of North Carolina, Greensboro, North Carolina.
Orel Examination Committee Members Thesis Direc
QML*+OJDate of Examinction
The author wishes to express her sincere appreciation to Dr. Pauline E. Keeney for her gracious help and understanding during the writing of this thesis.
She also wishes to thank Dr. TAiitfield Cobb, Kiss llarguerite Felton, Dr. Hildegarde Johnson and Mrs. Alice '.Tillinghem for their help- ful suggestions and encouragement; Dr. Thomas Donnelly of the Computation Center at The University of North Carolina for his help in the programing for Univaoj Lft-s. Frances Buchanan, lfi.88 Betty Ann Cagle, 13.3s Rosalind Ratchford and 10.88 Faye Tart for their help with tho testing and evalua-
tions; Dr. H. Y. Jennings of State College, Dr. Lee Waylaid of Dan River Mills, Inc. and Dan River Mills, Inc. for procuring the fabrics used in this study.
CHAPTER - ''-■- B
I. INTRODUCTION 1
II. RBVIHf OF LITERATURE 4
Resin Treatments for Wash and '.Year Properties 4
Definition 5 Wrinkle-Resistant Finishes 5 Fabric Softeners ?
Definition and Purpose
History of Fabric Softeners 7
Quaternary Cationic Fabric Softeners Fabric Softeners for Consumer Use
III. PROCEDURE n
Selection of Fsbric Softeners H
Selection and Preparation of Fabrics 11
Fabric Tests iVashing Procedure and Evaluation of the Surface
IV. PRESENTATION OP DATA 18
Fabric Construction 1°
Performance of Fabrics Before Experimentation 19
V CHAPTER PAGE Dimensional Change 20 Tear Resistance 25 Crinkle P.ecovery 30 Stiffness 35
Evaluation of the Surface Appearance 41
V. SUlOttRY AND CONCLUSIONS 47
APPENDIX A. Computer Programs for the Statistical Analysis
of Data 55
I. Computer Program for the Statistical Analysis of Data for Dimensional Change, Tear
Resistance, './rinkle Recovery, and
II. Conputer Program for Statistical Analysis
of Surface Appesrrnce Ratings 58
APPENDIX B. Analysis of Variance Tables for Dimensional
APfEr.DIX C. Analysis of Variance Tables for Tear Resistance . . .
APPENDIX D. Analysis of Variance Tables for Wrinkle Recovery . . 74
APPENDIX E. Analysis of Variance Tables for Stiffness APPENDIX F. Analysis of Veriance Tables for Surface
I. Softeners Found in Major Chain Food Stores 11
II. I'.Iean Results of Fabric Construction Tests 18
III. Lfean Results of Performance 19
IV. Differences in Fabrics as Indicated by Dimensional
Change 20 V. Comparison of Febric Softeners as Indicated by
Dimensional Change VI. Comparison of Treatments as Indicated by Dimensional
VII. Differences in Fabrics as Indicated by Tear Resistance . . 25 VIII. Comparison of Fabric Softeners as Indicated by Tear
Resistance IX. Comparison of Treatments as Indicated by Tear
Resistance 27 X. Means of bounds of Tear Resistance at the First
Interval in the »Varp Direction 30 XI. Differences in Fabrics as Indicated by Crinkle Recovery . . 31 XII. Comparison of Fabric Softeners ns Indicated by '.Vrinkle
XIII. Comparison of Treatments as Indicated by wrinkle
XIV. lueans of the Degrees of ".Vrinkle Recovery at the
XV. Differences in Fabrics as Indicated by Stiffness 36
XVI. Comparison of Fabric Softeners as Indicated by
XVII. Comparison of Treatments as Indicated by Stiffness .... 39
XVIII. ^ieans of Stiffness in Inches at the Third Interval
in the Filling Direction 41
XIX. Differences in Fabrics os Indicated by Surface
Appearance Ratings XX. Comparison of Fabric Softeners as Indiceted by
Surface Appearance Ratings XXI. Comparison of Treatments as Indicated by Surface
Appearance Ratings 44
XXII. Differences in Surface Appearance Ratings Given by
the Three Judges 45
XXIII. Analysis of Variance for Dimensional Change -
First Interval 63
XXIV. Analysis of Variance for Dimensional Change -
Third Interval 64
XXV. Analysis of Variance for Dimensional Change -
Sixth Interval 65
XXVI. Analysis of Variance for Dimensional Change -
Twelfth Interval XXVII. Analysis of Variance for Dimensional Change -
TA3LB XXVIII. XXIX. XXX. XXXI. XXXII. XXXIII. XXXIV. XXXV. XXXVI. XXXVII. XXXVIII. XXXIX.
Analysis of Variance for Tear Resistance - Before Laundering Analysis of Variance for Tear Resistance -
First Interval Analysis of Variance for Tear Resistance -
Third Interval Analysis of Variance for Tear Resistance -
Sixth Interval Analysis of Variance for Tear Resistance -
Twelfth Interval Analysis of Variance for Tear Resistance -
Twenty-fourth Interval Analysis of Variance for Wrinkle Recovery -
Before Laundering Analysis of Variance for Wrinkle Recovery -
First Interval Analysis of Variance for Wrinkle Recovery -
Third Interval Analysis of Variance for Wrinkle Recovery -
Sixth Interval Analysis of Variance for Wrinkle Recovery -
Twelfth Interval Analysis of Variance for Wrinkle Recovery -
Twenty-fourth Interval PAGE 68 69 70 71 72 73 74 75 76 77 78 79
TABLE XL. XLI. XLII. XLIII. XL1V. XLV. XLV1. XLVII. XLV1II. XLIX. L. LI.
Analysis of Variance for Stiffness - riefore
Laundering Analysis of Variance for Stiffness - First Interval . Analysis of Variance for Stiffness - Third Interval . Analysis of Variance for Stiffness - Sixth Interval . Analysis of Variance for Stiffness - Twelfth Interval Analysis of Variance for Stiffness - Twenty-fourth
Interval Analysis of Variance for Surface Appearance Ratings - Before Laundering Analysis of Variance for Surface Appearance ratings - First Interval Analysis of Variance for Surface Appearance Ratings - Third Interval Analysis of Variance for Surface Appearance Ratings - Sixth Interval Analysis of Variance for Surface Appearance Ratings - Twelfth Interval Analysis of Variance for Surface Appearance Ratings - Twenty-fourth Interval ix PAGE 80 81 82 83 84 85 86 87 89 90 91
1. Differences in Fabrics as Indicated by Dimensional
Change 2. Comparison of Fabric Softeners as Indicated by
Dimensional Change 3. Comparison of Treatments as Indicated by Dimensional
Change 4. Differences in Fabrics as Indicated by Tear Resistance . . . 5. Comparison of Fabric Softeners as Indicated by Tear
Resistance 6. Comparison of Treatments as Indicated by Tear Resistance . . 7. Differences in Fabrics as Indicated by Wrinkle Recovery . . . 8. Comparison of Fabric Softeners as Indicated by Vfrinkle
Recovery 9. Comparison of Treatments as Indicated by .Vrinkle Recovery . . 10. Differences in Fabrics as Indicated by Stiffness 11. Comparison of Fabric Softeners as Indicated by Stiffness . . 12. Comparison of Treatments as Indicated by Stiffness 13. Differences in Fabrics as Indicated by Surface
Appearance Ratings 14. Comparison of Fabric Softeners as Indicated by Surface
Appearance Ratings PAGE 21 23 24 26 28 29 32 34 34 37 38 40 43 43
xi FIGURE PAGE
15. Comparison of Treatments as Indicated by Surfece
Appearance Ratings 46 16. Differences in Surface Appearance Ratings Given by the
With the advent of synthetic fibers there was a decrease in the consumption of cotton fabrics. Cotton manufacturers, perceiving a de- cline in the use of cotton, attempted to find new ways to produce fabrics with as desirable crease and wrinkle resistant properties as those found in fabrics produced with synthetic fibers. After extensive research, synthetic finishing resins were produced to fulfill partially the desired requirements. These resins caused fabrics to lose their pliability, softness and strength. As early as the 1930's the textile industry be- gan using cationic fabric softeners to increase the pliability and strength of fabrics with resin finishes applied to themj however, the effectiveness of these softeners was lost after several washings.
Fabric softeners are no longer limited to industrial use. The consumer may purchase fabric softeners on the retail market to maintain the desired softness in garments and household products. Fabric soften- ers have been on the retail market for about seven years, but only recently have large producers of softeners been promoting their products with nationwide advertising campaigns. The consumer purchasing a fabric
softener will find a number of different brands from which to choose. With this variety, some confusion may exist as to which product is most
suitable for the desired results.
The purpose of this thesis was to study four fabric softeners available for consumer use. The two major objectives of tho study were:
first, to determine the degree of effectiveness of each fabric softener in maintaining the original surface appearance of the selected fabrics} second, to determine any effect of the fabric softeners upon the physi- cal properties of the fabrics such ss» stiffness, wrinkle recovery and tearing strength. The null hypotheses established to test these objec- tives arei
1. There are no differences in surface appearance between the fabrics treated with fabric softeners and those not treated with a softener.
2. There are no differences among fabric softeners in maintaining surface appearance of the fabrics.
3. There are no differences in physical properties between fab- rics treated with a fabric softener and those not treated with a softener.
4. There are no differences among the fabric softeners ts indi- cated by the physical properties of the fabrics.
This study was limited to the use of four brands of softeners which were in consumer use in the vicinity of Greensboro, North Carolina. The effectiveness of the softeners was determined by surface appearance evaluations and results of physical testing after the application of the softeners to three fabrics. These fabrics, obtained from one manufac- turer, differed in finish. One fabric had no finish othor than bleach- ing, mercerizing and other regular mill finishing treatments. The other two fabrics were finished with two resin treatments currently being applied to wash and wear fabrics. Evaluations of surface appearance and physical properties were made after the first, third, sixth, twelfth, and twent y-f ourth 1aund er ing s.
The remainder of the study is divided into four chapters. Chapter II is the review of literature which includes! (l) the history and definition of wash and wear and the types of wash and wear finishes used,
cationic softeners and consumer use. Chapter III describes the proce- dure for the selection of fabric softeners, selection and preparation of the fabrics, fabric tests, washing procedure and evaluation of the appearance and the statistical analysis. Chapter IV is the presentation and interpretation of the data found after performance of tests pertinent to the evaluation of the softeners. Chapter V contains the summary and conclusions of the study.
REVI&T OF LITERATURE
The "finishing operation" in the textile industry refers to any process applied to greige goods to produce a more desirable product. Finishes referred to as "additive finishes" are those applied to the
fabric or chemically added with the fibers to give the fabric some spe- cial effect. Some of these finishes would include water-repellent, flane-resistant, softening and crease-resistant finishes.
RESIN TREATMENTS FOR MSH ALTO 'flEAR PROPERTIES
Resin treatments were first introduced into the textile industry in the early 1930's to impart wash and wear characteristics including those of improved dimensional stability, wrinkle resistance and "hand"
of fabrics.2 By 1957 two billion yards of cotton were treated with
these resins. In 1960 cotton fabrics constituted sixty-three per cent of the wash and wear fabrics sold in the United States. Nearly two billion yards of fabrics were produced with wash and wear finishes and
lAnthony M. Schwartz, James W. Perry, Julian Berch, Surface Active Agents and Detergents Volume II (New York» Interscience Publish- ers, Inc., 195877 p. 255.
Robert M. Reinhardt, Russell M. H. Kullman, Harry B. Moore and J David Reid, "Aftermercerization of Wrinkle-Resistant Cottons for Improved Strength and Abrasion Resistance," American Dyestuff Kegortgr
"Wash and wear" has many definitions. The American Society for Testing Materials has defined it as:
A generic term applied to garments which satisfactorily retain their original neat appearance after repeated wear and suitable home laundering with little or no pressing or ironing.4
There are a number of chemioal resins used to impart wash md wear properties to fabrics. One of the most important groups are nitro- gen bases chemically combined with formaldehyde, known as N-methylol compounds which would include dimethylol urea, dimethylol ethylene urea, triazones, melamine formaldehyde, epoxides, and combinations of each of these finishes.5 Only the two finishes used in the study are discussed
Dimethylol ethylene urea (DMEU) is one of the most important of the N-methylol resins. DMEU imparts wrinkle resistant properties to fabrics by means of a cross-linking reaction with the cellulose by
Francis Burr, "Ironing Out Wash-and-Vfear Wrinkles," Chemical
■Teek, (September 23, 1961), p. 47.
4American Society for Testing Materials Committee D-13, ASTM
Standards on Textile Materials (Philadelphia: American Society for Testing Materials, 1961J, ASTM Designation: D 123-60, p. 44.
5A. C. Nuessle, "Creaseproofing Agents for ,Yash-and-Wear Finish-
changing the elasticity of the fiber.6 Fabrics finished with D1.Q3U have
a soft "hand," high wrinkle resistance without excessive strength losses and superiority in chlorine resistance; however, such fabrics are sub- ject to acid hydrolysis.
Triazone has been used commercially since early 1950. This cross- linking resin is less susceptible to chlorine damage and acid hydrolysis than is DMEU; for this reason triazone is used more for white fabrics. This finish is susceptible to discoloration and odor formation at high curing temperatures.
Chlorine retention is an important factor in wash and wear fin- ishes.
The resin treated cotton fabric acquires an ability to pick up chlorine from a hypo-chlorito bleach bath and form chloroamides. The chloroamides are unstable chemical compounds which may decompose at the temperature of ironing with a liberation of traces of hydro- chloric acid. It is the release of this acid during ironing that impairs the strength of a bleached, wash/wear fabric.8
Because there is a decrease in strength caused by application of resins, surfactants in the form of lubricants, softeners and thermo- plastic materials are added to the resin bath to decrease this loss.9
6j. G. Frick, Jr., 3. A. Kottes Andrews, and J. David Raid, "Effects of Cross-Linkage in Wrinkle-Resistant Cotton Fabrics," Textile Research Journal, (July, I960), p. 495.
to Wash p. 32
7Burr, op. cit., p. 48; and Sanford P. Young, "A oilman's Guide
-Wear Fin"ishe7," Modern Textiles Magazine, (October, 1961),
8Young, ibid., pp. 32, 57. 9Reinhardt, loc. oit.
Definition and Purpose
Fabric softeners belong to a group of chemicals known as sur- factants. This widely accepted word "surfactant" comes from the con-
traction of the phrase surface active agent.10
Probably the best definition for surfactants is that of vrater- soluble compounds which in moderate concentrations, for instance, in a 1% solution, reduce the surface tension of water to half or less of its original value. Since the surface of pure water is approximately 72 dynes per cm, a 1$ solution of the surfactant should have a tension of less than 36 dynes .... It is obvious that the usual function of a surfactant is to assist in maintaining the surface of interface between two phases, and thus to support wetting, penetrating, foaming, emulsifying, and dispersing.
A surfactant is formed by combining a water-soluble chemical group with an oil-soluble group so that the final product will have surface activi-
ty.12 Some surfactants would include: soaps, detergents, shampoos,
water-repellent finishes, softening finishes, and antistatic finishes.
History of Fabric Softeners
The textile industry has been using fabric softeners since the 1930's. They first began using them on rayon fabrics to give them a
softer "hand" and better draping qualities.13 Today in the textile in-
10Schwartz, op_. oit., p. 3.
nSamuel B. LIcFarlane (ed.), Technology of Synthetic Fibers (New
York: Fairchild Publications, Inc., 1953;, pp. 298-9.
12Armour Ethoxylated Chemicals, (Armour Industrial Chemical
Company, n.d.), p. 1.
13Harold L. Ward, "Textile Softeners for Home Laundering," Journal
dustry four types of fabric softeners are usedj (l) anionic; (2) quater- nary cationios; (3) non-quaternary cationics; and (4) nonionic compounds. Before those softeners were produced oil and wax emulsions and sulfonated gylceride fats were used as softeners. *
Quaternary Cationic Fabric Softeners
Most of the fabric softeners produced for consumer use are of the quaternary cationic type. This review deals with this type only, since the study made was on retail fabric softeners.
These fabric softeners work on the principle that the positively charged portion of the fabric softeners are attracted to tho negatively charged fabrics and form a coating on the filaments in tho fibers. This lubrication adds softness and allows the fibers to slip over each other thus reducing wear and increasing the life of the fabric. 15
The positive portion of the molecule containing the nitrogen and the long fatty hydrocarbon chains attaches itself, by virtue of the cationic properties of the nitrogen, to surfaces which are generally negative by comparison. This attachment is called "substantivity"
and is an electrochemical bonding or filming action which holds the high molecular weight cation closely to the individual fibers.
Because of this substantivity the required amount of softener depends on the number of pounds in the wash load rather than on the amount of water in the rinse water.*'
14Schwartz, op_. fTt., pp. 262-3.
15Technical Data Bulletin, (Texize Chemical, Inc., n.d.), p. 1. 16Arquad 2HT Fabric Softener and Conditioner, (Armour Industrial
Chemical Company, I960), p. 2.
l7"Home Laundry Fabric Softeners," (New York: Jane Ashley Home
The benefits derived from using a fabric softener include| softer fabrics, easier ironing, fewer wrinkles, faster drying, sanitizing and anti-static properties.18
Fabric Softeners for Consumer Use
Fabric softeners are applied to fabrics by many of the textile manufacturers. After a f ew launderings they are washed out of the fab- ric but the consumer can obtain the same effect by use of a commercial fabric softener.19
The production of fabric softeners for consumer use is relatively new. In 1955, sales for all brands amounted to half a million dollars. The sale of fabric softeners is growing at a rate of twenty-five per cent a year and it is estimated that by the mid-1960's it will be a fifty
21 million dollar a year business.
All brands of fabric softeners now on the retail market are based on the same general chemical compounds. Most consist of dialkyl quater- nary ammonium salts in an alcohol and water solution.
Typical formulai 75$ cationic surface-active agent (usually a quaternary ammonium chloride or sulfate) 18$ isopropanol and 7% water. This paste is further diluted with wetting agents (0.5-1$), odorants, tints, bluing, and the like. Active ingredients percent- age in the finished softener usually ranges from 3 to 8/..*
18Arquad 2HT Fabric Softener and Conditioner, op. cit., pp. 3-4. 19Ward, loc. cit.
20"Soft Touch is Tough to Sell," Chemical Week, (July 30, 1955),
21"Sales Spurt Puts New Zip Into Fabric Softeners," Chemical .Veek,
(December 30, 1961), p. 36.
10 The suppliers of raw material are numerous and highly competitive. Some of the main firms selling the basic softener formulation are: Archer- Daniels-Midland Company, Armour Industrial Chemical Company, Foremost Food and Chemical Company, General Kills Chemical Division, and Harshaw Chemical Corporation.23
Manufacturers of fabric softeners were confronted with two problems when the market opened. First, fabric softeners required an additional rinse in washing. Manufacturers had to conceive ways to point out to the consumer the benefits and values of this extra step.2* An additional
rinse is required because some soaps and detergents combine with fabric softeners forming an insoluble curd deposited on the fabric. 5 Secondly,
the cost was a problem. Since the average cost of a fabric softener was between three and four cents for an average wash load this was not as great a problem as the extra-step. 26
23" Sales Spurt Puts New Zip Into Fabric Softeners," oo_. cit., p. 36-7.
24"Soft Touch is Tough to Sell," loc cit. 25Technical Data Bulletin, op_. cit., p. 2.
26"Sales Spurt Puts New Zip Into Fabric Softeners," op_. cit.,
Selection of Fabric Softeners
The fabric softeners used in the study were brands sold commer- cially in the vicinity of Greensboro. The four softeners selected were those appearing on the shelves of each of four major chain food stores surveyed (Table I).
SOFTMBRS FOUND IN LIAJOR CHAIN FOOD STORES
Ma j or Food Stores Fabri c softeners
One Two Three Four Five Six Seven
A X X X X X X
B X X X X X
C X X X X X X
D X X X X X
Selection and Preparati on of Fabrics
The fabrics used in this study were given by Dan River Mills, Incorporated of Danville, Virginia. Three twenty-five yard lengths of approximately 85 x 74 print cloth were used for the study. Sample A was treated with a triazone finish, Sample B was treated with DMEU and Sample C was not treated with a resin finish. Each sample was cut into two groups marked as I and II. From these two groups forty squares 16" x 16" were cut and coded, using random sampling. Fifteen of these squares were used for rating surface appearance, the other twenty-five
12 squares were washed and removed for physical testing at predesignated washing intervals.
All the samples in each of the six groups of fabrics were coded to differentiate the control samples and those treated with each of the four softeners.
The following measurements were used to indicate the similarities or differences in the fabric construction as influenced by manufacturing procedures.
Fiber length was determined by removing a yarn from the fabric and untwisting until individual fibers could be removed without breaking. Those fibers were measured on a slightly oiled metal ruler. Three measurements were taken from both the warp and the filling yarns to obtain a mean length in inches for the fibers used in the warp and filling yarns.
Twist per inch was determined by means of tho twist counter manufactured by the United States Testing Company Incorporated. The test procedure followed was that recommended by the American Society for Testing Materials.1 The test determines the number
of turns per inch in the yarn and the direction of the twist. The principle is to remove all the twist from a given length and put the twist baok into the yarn until the original length is
xAmerican Society for Testing Materials Committee D-13, ASTM
Standards on Textile Liaterials (Philadelphia: American Society for Testing Mate"riaTsTT96i;, Test Designation. D 1422-59T, pp. 587-9.
13 obtained. Five tests were made on tho warp yarns and five on the filling yarns. The results reported tor each direction were a mean of these five tests.
Thread count was determined by the procedure recommended p
by the American Society for Testing Materials. A micrometer was used to count the warp and filling yarns per square inch. Two counts were made in each direction and an average taken as the final results for warp count and filling count.
Yarn number or the size of the yarns in relation to the weight, was determined by means of the Roller-Smith Univsrsal Yarn Numbering Balance. In this method thirty-six inch lengths of yarn were removed from, the fabric weighed on the balance. The means of three tests made on tho warp were reported as the yarn number of that direction. The same number of tests were made on the filling yarn.
Weight per square yard was determined by a modification of the method recommended by the American Society for Testing Mate- rials.3 Three 2x2 samples were weighed on a gram balance after
drying to remove the moisture. The weight was obtained by using the formula:
/ , Weight of sample in grams x Sq. inohes/sq. yard
•/ I* ya* Number of square inches Grams/ounce
The mean of the three tests was reported as the ounces per square yard of the fabric.
2Ibid., Test Designation: D 1910-59T Sections 20-23 pp. 823-4.
14 The following tests were made to determine the serviceability of the fabrics. These tests were made on the original fabric and on swatches of the fabric removed after the first, third, sixth, twelfth, and twenty-fourth washing intervals.
Tear resistance was used to determine the mean force re- quired to continue a tear starting from a cut in the fabric. The instrument used was a tear tester of the falling-pendulum type manufactured by Thwing-Albert, Elmendorf Tearing Tester $6-400. The testing procedure followed was that established by the Ameri- can Society for Testing Materials.4 The means of five warp and
of five filling specimen were reported as the tear resistance in the two directions.
Dimensional change was used as the measure of shrinkage in the warp and filling threads. The test squares were cut and mark- ed with squares measuring fifteen by fifteen inches. Following the launderings, a mean of three measurements was taken and re- ported as the dimensional change for the warp and filling direc- tions.
Wrinkle recovery tests were made using the method
recommended by the American Association of Textile Chemists and Colorists.5 This test determines the recovery of fabrics from
creasing. A sample is creased under controlled conditions of time and weight, allowed to hang in the Monsanto Wrinkle Recovery
Void., Test Designation! D 1424-59, p. 597-601.
William D. Appel, 1961 Technical Manual of the American Associa- tion of Textile Chemists anTTolorists Volume XXXVII. (New York, Howes
Tester for a stated period of time before the recovery ongle is measured. The means of six samples in the warp direction and of six in the filling direction were totaled and reported as the wrinkle recovery.
Stiffness of the cloth was determined by the cantilever method as recommended by the American Society of Testing Materi-
als.6 The drape-flex stiffness tester manufactured by Fabric
Development Tests was used for the evaluation. The test was em- ployed to determine the drape stiffness which measures how much a fabric drapes under its own weight. The mean of eight tests was reported as the stiffness in inches of overhand in both the warp and filling directions.
Washing Procedure and Evaluation of the Surface Appearance
The test methods for these procedures are based on the test method recommended by the American Association of Textile Chemists and Colorists.7 The washing machine used was a small size reversing wash
wheel type commercial washer manufactured by the American Laundry Liachine Industry. A five pound load consisting of test samples plus fabric for extra weight was washed for ten minutes at 140 degrees Fahrenheit with a six inch water level. The samples were given three four-minute rinses using a seven inch water level at 105 degrees Fahrenheit. The fabric softeners were added to the final rinse. The samples were removed from the washer, hung with the warp in a vertical position and allowed to
6American Society for Testing Materials Committee D-13, op_. cit.,
Test Designationi D1388-55T, pp. 581-8.
drip dry. The pH of the water vras checked at predesignated periods by a pH meter manufactured by Analytical Measurements Incorporated.
The purpose of the evaluation of the surface appearance was to determine the retention of the original appearance after specified laun- derings. The samples were rated under standard lighting conditions and given numerical ratings based on standard plastic replicas manufactured by the Monsanto Chemical Company. A panel of three members evaluated samples from each of the six fabric groups at each testing interval. The fifteen samples in each fabric group evaluated consisted of three control samples (those laundered with no softener) and three laundered using each of the four softeners.
The data from tests of tear resistance, dimensional change,
wrinkle recovery and stiffness were analyzed for any significant differ- ences between fabrics, treatments and the fabrics times the treatments.
The data from tests of surface appearance were analyzed for any significant differences between fabrics, treatments, judges, fabrics times judges, fabrics times treatments, treatments times judges and fabrics times treatments times judges.
The F distribution was used to test each source of variation. The sum of squares was caculated for each source of variation and divided by the appropriate degrees of freedom to produce the mean square. To obtain the F values, each mean scuare was divided by the appropriate experimental error. The five per cent and one per cent level of signifi- cance were arbitrarily chosen for rejection of the hypotheses.
The data were processed on the Remington Rand Una vac 1105 at The Computation Center at The University of North Carolina. The programs used to process these data are found in Appendix A.
PRESENTATION OF DATA
I. FABRIC CONSTRUCTION
Before experimentation all three fabrics were tested to determine the fiber length, yarn number, twist count, thread count, and weight. These tests were made to be certain that the basic construction was the same for all three fabrics. The mean results of these tests on the three fabrics are shown in Table II. Tho slight differences between the labo- ratory tests and the data supplied by the manufacturer were considered due to differences between specifications and the manufactured fabrics.
LiEAN RESULTS OF FABRIC CONSTRUCTION TESTS
Fiber length Twist Weight
Fabric (Inches) Yarn number (Inches) (Oz/
Warp Filling Warp Filling Warp Filling Warp Filling sq/yd)
A 0.9 B 0.9 C 0.8 1.0 1.0 1.1 43's 41's 44's 32's 32's 31's 29Z 27JS 26Z 22S 21S 20S 82 83 83 74 74 75 3.2 3.3 3.1 Specifications given by the manufacturer
40's 30's 85 74 3.1
The principle differences which did exist in the fabrics were in the finish applied by the manufacturer. Fabric A was treated with a triazone finish, Fabric B with dimethylol ethylene urea (Dl.ffiU), Fabric C had only usual mill treatments in preparation for finishing. No resin finishing treatment was applied to Fabric C. Fabrics A and B were San- forized.
II. PERFORMANCE OF FABRICS BEFORE EXPERIMENTATION
The Fabrics A, B, and C were tested to determine tear resistance, wrinkle recovery, and stiffness before any laundering treatment was applied. Mean results of the tests are given in Table III.
MEAN RESULTS OF PERFORMANCE Fabric Tear resistance
(Rounds) iTrinkle recovery (Degrees) Sti (Inches i'»arp ffness overhang)
Warp Filling Filling
A B C 1.87 1.92 1.70 1.36 1.19 1.40 257 264 118 1.51 1.73 1.93 1.41 1.49 1.83 Mean 1.58 1.56 213 1.72 1.58
The fabric with no resinous finish, Fabric C, was lower in warp tear resistance end wrinkle recovery than either Fabrics A or B. The filling tear resistance of Fabric B was slightly less than the filling tear resistance of Fabric C. The stiffness of Fabric C was higher than either of the resin finished fabrics. This would indicate that the fab- rics with resinous finishes were softer and superior in tear resistance and wrinkle recovery.
III. PERFORMANCE OF FABRICS AFTER LAUNDERING
In this section of the study, comparisons of the effectiveness of the four fabric softeners were based upon the means of tests applied to each of the three fabric types. Comparisons made between fabrics to which no softener had been applied and those treated with a softener
20 were based upon the mean of means of the three fabrics. This applied to tests made both before laundering and those made at each testing inter- val.
There were differences in the shrinkage of the three fabrics. >7arp dimensional change of Fabrics A and B were slight and well below the 1.0 per cent established for Sanforized fabrics. Fabric C had the greatest shrinkage of all the fabrics. The shrinknge ranged from 2.50 per cent at the first interval to 4.16 per cent at the twenty-fourth interval. In the filling direction the fabric with the least shrinkage at all intervals was Fabric B. Fabric C was also the highest in shrink- age in the filling direction (Table IV, Figure l). These changes were expected since Fabric C was not Sanforized. These differences in the fabrics were found to be statistically significant at the one per cent level at all the intervals (Appendix B).
DIFFERENCES U FABRICS AS BTOICAffHD BY DILMSIONAL CHANGE
Interval Per cent Warp Change Per cent Filling Change
Fabric fabric A B C A B C 1 -0.18 -0.01 -2.50 -0.76 -0.47 -7.67 3 0.22 0.09 -2.89 -0.88 -0.59 -8.29 6 0.10 -0.04 -3.30 -1.09 -0.65 -8.43 12 0.00 -0.20 -4.03 -1.22 -0.72 -8.17 24 0.29 0.00 -4.16 -1.02 -0.49 -7.25
The effect of the fabric softeners on the dimensional change varied little between softeners. In the warp direction there was less
3 fa •O 0 fa ID C\J T) 10
1EH H O § 13 O M CO >H fa + 5 CH O O I <no o •H
•9Li fa I* [X. fc CM 0 fa © ■a to © <o EH w o i t> i I rH W M EH o M Q CO < CO o
22 shrinkage than in the filling direction. There was continuous shrinkage up to the sixth interval but the fabrics began to show less shrinkage at the twenty-fourth interval (Table V, Figure 2). The differences in the shrinkage were not statistically significant at any of the laundering intervals (Appendix B).
COMPARISON Oi'' FABRIC SOFTENERS AS INDICATED BY DILI3SSI0NAL CHANGE
Per cent warp change Per cent filling change
Interval Softeners Softeners
One Two Three Four One Two Three Four
1 -0.84 -0.64 -0.74 -0.89 -3.29 -3.02 -2.42 -3.16
3 -1.03 -1.01 -0.89 -0.86 -3.34 -3.42 -3.12 -3.30
6 -1.20 -1.24 -1.03 -1.01 -3.39 -3.59 -3.38 -3.49
12 -1.59 -1.23 -1.64 -1.38 -3.40 -3.42 -3.26 -3.47
24 -1.39 -1.27 -1.39 -1.16 -2.87 -3.10 -2.87 -3.21
Comparing the dimensional change of fabrics treated with the four softeners and those not treated with a softener it was found that there was less shrinkage in the fabrics which did not have r. fabric softener added to the final rinse. This was true in both warp and filling direc- tions (Table "VI, Figure 3). This difference in shrinkage was significant
COliPARISON OF TREATMliKTS AS INDICATED BY DIMENSIONAL CHANGE Interval Per cent warp change Per cent filling change No softener Softeners No softener Softeners
1 -0.76 -0.78 -2.93 -2.97
3 -0.52 -0.95 -3.08 -3.30
6 -0.91 -1.12 -3.09 -3.46
12 -1.21 -1.46 -3.33 -3.39 24 -1.21 -1.30 -2.53 -3.01
o o > rt so 3 Co CD C to S3 t- P 9 >=] § **! a te i CO n FO a l-H a O CO c :,: 0) CO CO CO co 1 o o o 0 // Hi M, Hj ft jr d- d- c+ <+ /i § § § <D / / S «/ >-• . CD CD a o MA to -1 1 -i 1 TTT ■q rt >-i ^ \ \ O
s§c co H i a i CD 1 1 1 1 tv3 i I | 1 1 * ' a t> O • 5" O § CO 1-3 0> 3 o CD 63 CD
i?t- o c EC 5 I cn i M CD a l-H £2
8« 1-3 O) p. ro p.
p- //o o / / ft / / a- CO / / S ° / / 3 1 1 a c+ / / 10) Ji 13 Y ' 1 CD 1 •"» 1 ' *
6* 1( M CT3 O H CD •*3
at the third, sixth, and twelfth intervals in the warp direction (Appendix B).
Tear resistance for the three fabrics was reported in pounds. In the warp direction Fabric B had the lowest tear resistance at all testing intervals except the original testing period when Fabric C was the low- est. Fabric A had the highest resistance at this interval, but in all other intervals Fabric C was the highest. In the filling direction Fab- ric B had the lowest resistance at all intervals. At all except the first interval Fabric C had the highest tear resistance (Table VII, Fig- ure 4). These differences between fabrics were statistically significant
at the one per cent level, at the first, third, sixth, twelfth, and twenty-fourth intervals in the warp and filling directions (Appendix C).
DIFFERENCES IN FABRICS AS INDICATED BY TEAR RESISTANCE
Interval Warp resistance Fill ing resi stance
(Pounds) (Pounds) A Fabrics B
AB C 0 1.87 1.70 1.19 1.92 1.36 1.40 1 1.90 1.73 2.04 1.98 1.36 2.36 3 1.91 1.79 2.25 1.96 1.48 2.60 6 2.11 1.92 2.49 2.11 1.62 2.49 12 1.95 1.88 2.44 2.00 1.58 2.77 24 2.04 1.93 2.40 2.13 1.72 2.78
Comparing the softeners by tear resistance of the fabrics, the warp direction of softener one was highest at all intervals except the twelfth. Softener four was lowest in tear resistance at all intervals. In the filling direction no one softener remained highest at any of the
26 SB ft.
3•a CM o ,-< I- D (0 Hi CO CD ID e , CO Pi ■ T3 ' o CM P-. CO • CM • CO CM • CM o • CM CO • r-4 pa o M ft, (a o H CO
sW H CD S3 o t-l Q
5CO o M ft. CO ra Q
six intervals (Table VIII, Figure 5). Differences in these softeners were statistically significant at the one per cent level at the first and third intervals in the warp direction and at the first interval in the filling direction. The differences were significant at the five per cent level at the twelfth interval in the warp direction and at the third in the filling direction (Appendix C).
COIPARISON OF FABRIC SOFTENERS AS INDICATED BY TEAt rtESISTAJCE interval Warp resistance Fi lling resistance
(Founds ) (Pounds)
One Two Three Four One Two Three Four 0 1.58 1.58 1.58 1.58 1.56 1.56 1.56 1.56 1 2.01 1.99 1.93 1.87 2.07 1.95 2.01 1.85 3 2.09 2.05 2.02 1.98 2.10 2.13 2.04 2.04 6 2.26 2.24 2.18 2.16 2.12 2.19 2.09 2.01 12 2.09 2.11 2.14 2.09 2.15 2.14 2.16 2.10 24 2.18 2.17 2.17 2.13 2.26 2.27 2.20 2.21
At all intervals in both the warp and filling directions fabrics treated with softeners had a higher tear resistance than those not treat- ed (Table IX, Figure 6). Differences in treatments were statistically- significant at all intervals (Appendix C).
COlJPARISGi ' OF Thii&TLiSf'
TS AS INDICATED BY TiAii i.iSSISTAl'iCE Interval Warp resistance
I 'illing resistance (Pounds)
Hosoftener Softeners IJO softene r Softeners 0 1 3 6 12 24 1.58 1.64 1.78 2.04 2.03 2.02 1.58 1.95 2.28 2.21 2.11 2.18 1.56 1.61 1.79 1.96 2.04 2.13 1.56 1.97 2.08 2.10 2.14 2.23
3H ■o o CM CO i-l u § © EH ■o Crt M « | *J K CO 3 (O (D
sU•H EH EH H to PQ in ta l-H M EH
aEH W H-l 03 PS. (a a o w CO <a 03 % 3, N C\J C\2 W
30 The interactions between the fabrics and treatments were found to be statistically significant at the first, third and twelfth intervals in the warp direction. They were significant at the first, third,
twelfth and twenty-fourth intervals in the filling direction (Appendix C, Tables XXIX, XXX, XXXII, XXXIIl).
In all cases when the interaction was significant the tear resist- ance of Fabric C was increased more when treated with fabric softeners than when no softener was added. Table X is an example showing a sig- nificant interaction.
MBHT8 OF POUNDS OF TSAR RESISTANCE AT THE FIRST INTERVAL III THE 7TARP DIRECTION
Bo softener Softeners
One Two Three Four
A B C 1.83 1.68 1.41 1.92 1.91 1.80 1.74 2.30 2.34 1.88 1.74 2.18 1.97 1.68 1.96 Wrinkle Recovery
The results of the wrinkle recovery tests were recorded in degrees of the recovery angle. According to Taube, Ross rnd Poole "wash and wear fabric" should have a crease recovery measurement of 275 degrees to
HU Katherine Taube, Enid S. Ross rnd Nad a D. Poole, "Use of Mod- ern Home Laundry Equipment I. Wrinkling Effects en Swatches of Present- Day Fabrics," American Dyestuff Reporter, (June 26, 1961}, p. 38.
There were differences in the angle of recovery for the three fabrics. At eaoh interval of testing; Fabric A had the highest recovery, and Fabric C had the lowest. The wash and wear finish applied by the nanuf acturer to Fabrics A and B was evident in the results of this test
at eaoh laundering interval (Table XI, Figure 7). The differences in the three fabrics were statistically significant at the one per cent level at all the testing intervals (Appendix D).
DIFFERENCES IB FABRICS AS INDICATED BY flRINKLE RECOVERY
Interval Fabrics (Degrees) A B C 0 257 264 118 1 259 256 148 3 258 256 164 6 261 255 172 12 264 258 174 24 265 259 177
In all cases the wrinkle recovery of the fabrics increased from tho original after laundering with the four fabric softeners. There was a range of a low of 218 degrees after the first washing interval to a high of 237 degrees after twenty-four washings. Softener number three was the lowest of the four softeners through the sixth washing but was the highest after the twenty-fourth laundering (Table XII, Fieure 8).
There were slight differences between softeners at each interval; how- ever, these were not great enough to show one softener superior to another. These differences were statistically significant at the twenty-fourth interval at the one per cent level (Appendix D).
32 Degrees 280 260 240 220 200 180 160 140 120 100 Fabric A -• Fabric B -0 Fabric C -A 3 6 12 Times Laundered 24 FIGURE 7
After each testing interval fabrics treated with a softener had a higher angle of recovery than did fabrics not treated with a fabric sof- tener (Table XIII, Figure 9). These differences were not large, but were statistically significant at the five per cent level at the third and twelfth intervals and the one per cent level at the twenty-fourth interval (Appendix D).
COMPARISON OF FABRIC SOFTENERS AS E4DICATED BY 'WRINKLE RECOVERY
One Two Three Four
0 213 213 213 213 1 223 223 218 220 3 228 228 224 228 6 229 233 226 232 12 231 234 234 232 24 234 235 237 235 TABLE XIII
COMPARISON OF TREATMENTS AS INDICATED 3Y ■JRINKLE RECOVERY
Interval No softener Softoners
(D egrees) (Degrees) 0 213 213 1 220 221 3 221 227 6 227 230 12 227 233 24 227 235
The interaction between the fabrics and the treatments were found to be statistically significant at the third, sixth and twenty-fourth intervals at the one per cent level (Appendix D. Tables XXXVI, XXXVII, XXXIX).
34 - • O 1 1 L co 01 u •P <D 4-1 a O m CO +> «H o n BB CO ■ ■ ■a CO X) Bfl Q 25 CO CO o EH Q ^ | cs w CO M en CO h< H E fa o o w o o 4 a i i i i 0 i IP u - U 3 S .G o EH EH fx, Lblih CO O CO CD +> 43 +J +5 CH 4H CH "M o o o o CO CO CO CO *o 6-1 R <l> fa w u O 03 CO CO •o CO w W
B9fa B CO fa i fa >H •H O CO §@ CO EH ►H. <c OJ o «; HH
i§O M O
Yftien Fabric B was treated with softener two the wrinkle recovery rating was higher than when it was treated with tho other softeners. These were the only two combined factors which were repeated in all three interactions. Table XIV is an example of this interaction.
MBABS OF TiiE DEGREES OF VKMKLE RECOVERY AT THE THIRD INTERVAL
No softener So fteners
One Two Three Four
A B C 256 251 154 264 256 164 261 260 164 254 254 164 257 257 172 Stiffness
The stiffness of the fabrics was decreased with washings. In the warp direction Fabric C was the highest at all intervals, Fabric B was the lowest. In the filling direction Fabric C was the highest at all intervals except at the twenty-fourth interval. Fabric A was the lowest at all intervals except the twelfth and twenty-fourth when Fabric B was lower. This indicates that Fabrics A and B were softer than Fabric C (Table XV, Figure 10).
These differences in fabrics in the warp direction were statisti-
cally significant at the one per cent level of probability at the first,
third, sixth and twelfth intervals. They were significant in the fill-
ing direction at the one per cent level at the third and twelfth inter-
vals and at the five per cent level at the first and twenty-fourth
36 In the warp direction fabrics treated with the four softeners at the first interval vcried from a low oi' 1.43 to a high of 1.52. At the other intervals the difference was no greater than .04 inches. In the filling direction the greatest difference occurred at the first interval where there was a variation of .08 inches. After tne twenty-fourth washing only .01 inches variation occurred (Table XVI, Figure 11). These differences in warp stiffness were statistically significant at the five per cent level, at the third, sixth and twenty-fourth intervals. (Appen- dix E).
DE-TERENCES IN FABRICS AS INDICATED BY STIFFNESS
Interval Warp stiffness Filling sti ffness (Inch es overhang) (Inches overhang)
A B C A B C 0 1.51 1.73 1.93 1.41 1.49 1.83 1 1.36 1.49 1.56 1.33 1.35 1.42 3 1.29 1.39 1.47 1.29 1.32 1.42 6 1.29 1.39 1.47 1.33 1.35 1.35 12 1.30 1.32 1.36 1.34 1.32 1.36 24 1.30 1.30 1.32 1.33 1.30 1.32 TABLE XVI
COMPARISON OF FABRIC SOFTMI ERS AS E.'DICATED BY STIFFNESS Interval Warp stiffness Filling s tiffness
(Inches overhang) (inches ovorhang)
One Two Three Four One Two Three Four 0 1.72 1.72 1.72 1.72 1.58 1.58 1.58 1.58 1 1.43 1.44 1.50 1.52 1.34 1.34 1.36 1.40 3 1.36 1.32 1.38 1.37 1.33 1.35 1.36 1.32 6 1.34 1.32 1.36 1.35 1.35 1.32 1.35 1.34 12 1.32 1.32 1.32 1.32 1.34 1.34 1.33 1.33 24 1.31 1.29 1.30 1.29 1.31 1.31 1.31 1.30
" S•o CM (D rH U a •o CO g
sij 55 10
£<D (D M 1 EH •H CO E-< >H to CO
3CO o M I*
38 •o N © CD rH U co
sEu ! G ■ M ►J EH M W CO © >H a 03 W OH ■ si «-
4• o o a 1 1 1 1 1 1 1 1 1 1 ID 1 1 1 <D U J> p U 3
8£3 o u u r. t. <D ID IS ID &5§
§ i■P +> CH C CH *H o o o o co co CO CO T3 OJ CO rH r< (D •a CO to CD •H EH l-H &H PS CO o o o co f- <o
or ! ••#
39 In tho warp direction fabrics treated with a fabric softener were lower in stiffness than those not treated with a softener in all cases except at the first interval. In the filling direction fabrics treated with the softeners were lower at all intervals (Table XVII, Figure 12). Those differences were statistically significant at the one per cent level, at tho third and twenty-fourth intervals in the warp direction and at the twenty-fourth interval in the filling direction. They were significant at the five per cent level, at the twelfth interval in the filling direction (Appendix E).
COITARISOII OF TREAT (EEFTS AS INDICATED BY STIFFNESS
Interval i/arp sti ffness Filling st iffness
(inches overhang) (Inches overhang)
No softener Softeners i.'o softener Softeners
0 1.72 1.72 1.58 1.58 1 1.46 1.47 1.39 1.36 3 1.43 1.37 1.36 1.34 6 1.36 1.34 1.35 1.34 12 1.33 1.32 1.35 1.33 24 1.34 1.30 1.34 1.31
The interactions between fabrics and treatments were found to be statistically significant at the five per cent level at the third and twelfth intervals in tho filling directions (Appendix E, Tables XLII, XLIV). In all cases when the interaction was significant Fabrics A and B had lower stiffness results when fabrics were treated with the fabric softeners than when no softener was added. Table XVIII is on example of this interaction.
IV. EVALUATION OF THB SURFACE APPEARANCE
Ratings from one to five given by the panel of three judges were based on tho Monsanto Standards for wash and wear fabrics. The ratings given the three fabrics laundered by the five different treatments were used to indicate the consumer acceptance of the specially finished fab- rics as compared with the same fabric with no special finish.'
MBUI8 OF STIFFNESS IN INCHES AT THE THIRD INTERVAL IN THE FILLING DIRECTION
No softener Softeners
One Two Three Four
A B C 1.30 1.30 1.48 1.30 1.30 1.40 1.28 1.36 1.40 1.29 1.35 1.43 1.26 1.30 1.41
Differences in tho three fabrics were more noticeable following laundering than at the initial examination period. The unlaundered sam- ples of Fabrics A, B, and C were given the highest ratings ranging from 4.8 to 5.0. At each of the other intervals Fabric B, with the DIJB'J fin- ish, had the highest ratings and Fabric C, with no wash and wear finish, the lowest. For this study ratings from 3.0 to 5.0 were selected to indicate fabrics meriting consumer acceptance as wash and wear fabrics. Fabrics A and B maintained ratings high enough to be considered wash and wear fabrics (Table XIX, Figure 13). The differences in the fabrics were found to be statistically significant at tho one per cent level at all
42 The evaluations of fabrics treated with each of the four fabric softeners ranged from a high of 4.9 to a low of 2.9. There was a large decrease in ratings at the first laundering interval. At all subsequent intervals this rating remained relatively consistent (Table XX, Figure 14). There were statistically significant differences among treatments
DIFFERENCES IN FABRICS AS INDICATED BY SURFACE APPEARANCE RATINGS
Interv al Fabri cs A B C 0 4.8 5.0 4.9 1 3.1 3.9 1.3 3 3.4 4.1 1.3 6 3.4 4.1 1.2 12 3.4 4.1 1.5 24 3.4 4.1 1.5 TABLE XX
COWARISON OF FABRIC SOFTENERS AS INDICATED BY SURFACE APPEARANCE RATINGS
One Two Three Four
0 4.9 4.9 4.9 4.9 1 2.8 2.9 2.8 2.9 3 2.9 2.9 2.8 2.9 6 2.9 2.9 2.7 2.8 12 3.0 3.0 3.2 3.2 24 3.0 3.1 2.9 3.0
at the five per oent level at the first and twenty-fourth intervals and at the one per cent level at the sixth and twelfth intervals (Appendix F). Although the differences among softeners were statistically signifi-
Ratings 5« \\—- 4
AFabric A -• 2 \ Fabric B -0 [ \ Fabric C -4 \ n 1 1 4
t ,■ 3 6 12 Times Laundered 24 FIGURE 13
DIFFERENCES IN FABRICS AS INDICATED BY SURFACE APPEARANCE RATINGS
Softener One • Softener Two O Softener Three--A Softener Four---0 3 6 12 Times Laundered FIGURE 14
COWARISON OF FABRIC SOFTENERS AS INDICATED BY SURFACE APPEARANCE RATINGS
44 to be effective. There vrere also statistically significant interactions between fabrics and treatments at the third, sixth, pnd twelfth inter- vals, but these interactions did not show any variation among the four softeners.
The fabrics treated with softeners and those not treated with softeners varied slightly in ratings. The fabrics treated with softeners had higher ratings except at the sixth interval (Table XXI, Figure 15). The differences in the treatments were not statistically significant at any of the laundering intervals.
COMPARISON OF TREATLO&ITS AS INDICATED BY SURFACE APPEARANCE RATINGS
Interval Ho softener Softeners
0 5.0 4.9 1 2.6 2.8 3 2.9 2.9 6 3.1 2.6 12 3.0 3.1 24 3.0 3.0
There vrere differences in the ratings given by the three judges at all intervals. Judge three always gave the highest ratings. In most cases Judge one gave the lowest ratings (Table XXII, Figure 16). These differences between judges were statistically significant at all the intervals at the one per cent level (Appendix F).
DIFFERENCES III SURFACE APPEARANCE RAT DIGS GIVES BY THE THREE JUDGES
One Two Three
4.8 5.0 5.0 2.5 2.5 3.3 2.6 2.7 3.5 2.6 2.7 3.3 2.6 2.7 3.8 2.6 2.7 3.8 0 1 3 6 12 24
46 Mo Softener—• Softeners 0 3 6 12 Times Laundered 24 FIGURE 15
C01.IPARISON OF TREATMENTS AS INDICATED BY SURFACE APPEARANCE RATINGS
Judge 1 -• Judge 2 -0 Judge 3 -4 3 6 12 Times Laundered 24 FIGURE 16
DIFFERENCES IN SURFACE APPEARANCE RATINGS GIVEN BY THE THREE JUDGES
The textile industry, recognizing the need of modern consumers for fabrics requiring less care, has produced many finishes to impart properties of crease and wrinkle resistance and also wash and wear char- acteristics to cotton fabrics. Fabric softeners were first applied to these resin treated fabrics to maintain the pliability, softness and strength of the fabrics.
In recent years fabric softeners have gained popularity as home laundering aids. Their value in maintaining softness in towels, rugs and other textile products has been recognized. It is thought that they might be of value in maintaining the appearance of fabrics treated for
ease of care and might also extend the serviceability of such fabrics by counteracting the damaging effect of the resin finishes.
The purpose of this study was to investigate the effectiveness of softeners upon the surface appearance and physical properties of fabrics. Four brands of fabric softeners were selected from those commercially
available. The test fabrics used were of a standard broadcloth construc- tion varying in finishing treatments, namely: Fabric A was treated with a triazone finish; Fabric B was treated with dimethylol ethylene urea
(D2S2U); and Fabric C had only usual mill treatments in preparation for finishing. The fabrics were laundered twenty-four times and tested at designated intervals to determine I
(1) The differences in surface appearance between the fabrics treated with fabric softeners and those not treated with a softener.
(2) The differences among the softeners in maintaining the surface appearance.
(3) The differences in physical properties between the fabrics treated with a fabric softener and those not treated with a softener.
(4) The differences among the softeners as indicated by the physical properties of the fabrics.
Laboratory tests and measurements usod to indicate the differences in the three test fabrics were dimensional change, tear resistance,
wrinkle recovery, stiffness and surface appearance. The data were tested for their significance at the five and one per cent levels by using an Analysis of Variance.
The differences in the finish of the fabrics contributed to dif- ferences in physical tests. Those were apparent in the fabric both before laundering and after laundering. In many cases the differences were due to the Fabric C which had no finish other than the regular mill finish. The differences among the fabrics were statistically signifi- cant for all physical tests performed.
Fabrics A. and B had loss shrinkage at all laundering intervals than the maximum for Sanforized fabrics in both the warp and filling di- rections. Fabric C had more shrinkage than the maximum for Sanforizing. There was less shrinkage of the fabrics laundered without a fabric sof- tener added to the rinse water than those treated with a softener. How- ever, this difference was not great enough to be statistically significant.
All three fabrics increased in tear resistance after laundering. Fabric C increased more than did Fabrics A and B. The fabrics treated
with a fabric softener increased in tear resistance slightly more than the fabrics not treated with a softener. This difference was not con- sidered to be of importance except in Fabric C where it was found that the addition of e fabric softener did increase the tear resistance.
Throughout all the laundering intervals Fabrics A and B maintain- ed the degrees of wrinkle recovery which would enable them to be consid- ered wash and wear fabrics. At none of the intervals did Fabric C have an angle of recovery equivalent to a wash and wear fabric. The wrinkle recovery angle of Fabric C did increase after laundering but this was as prevalent in the samples laundered without the softener as in those treated with a softener.
The stiffness of all three fabrics was decreased after the laun- derings but this was not found to be due to the addition of the fabric softeners.
In only one of all the physical tests performed was it found that a fabric softener was of any benefit. This was in the tear resistance of Fabric C which was increased by the use of a fabric softener. In no cases was it found that one fabric softener was superior to another.
From the evaluations of the surface appearance it was shown that Fabrics A and B maintained ratings sufficient for wash and wear fabrics. Fabric C did not maintain a rating above 1.5 after the initial judging. There were no differences found among the four softeners; however, there were some differences found between fabrics not treated with a softener. These differences were so slight that thoy would not make any difference to consumer use.
50 The conclusions reached from this study were that fabric softeners did not holp to maintain the surface appearance end physical properties of fabrics treated to have wash and wear properties. There were no dif- ferences in the effectiveness of the fabric softeners selected.
Since fabric softeners have increased in production and sales in recent years it is suggested that further study be made of the applica- tion of fabric softeners to determine their true value. It is suggested that fabric softeners be applied to knit or pile fabrics rather than flat surface fabrics such as used in this study.
Appal, William D. 1961 Technical Manual of the Americen Association of Textile Chemists md Golorists VolumelCQCVlI. Hew York: Howes Publishing Co., Inc., 1961.
American Society for Testing Materials Committee D-13. ASTM Standards of Textile Materials. Philadelphia! American Society for Testing Materials, 1961.
McFarlane, Samuel B. (ed.). Technology of Synthetic Fibers. New Yorki Fairchild Publications, Inc., 1953.
Ostle, Bernard. Statistics In Research. Amers, Iowai The Iowa State College Press, 1954.
Schwartz, Anthony 11,, James W. Perry and Julian Berch. Surface Active Agents and Detergents Volume II. New York: Interscience Publishers, Inc., 1958.
(Talker, Helen H, and Joseph Lev. Statistical Inference. New York: Henry Holt and Company, 1953.
Burr, Francis. "Ironine Out Wash-and-Wear Wrinkles," Chemical Week, (September 23, 1961), pp. 47-8.
Frick, J. G., Jr., B. A. Kottes Andrews, and J. David Reid. "Effects of Cross-Linkage in Wrinkle-Resistant Cotton Fabrics, Textile Research Journal, (July, I960), pp. 495-504.
Nuessle, A. C. "Creaseproofing Agents for Wash-and-,/ear Finishing," Textile Industries, (October, 1959), pp. 116-27.
Reinhardt, Robert II.. Russell K. H. Kullman, Harry B. Moore and J. David Reid. "Aftermercerization of Wrinkle-Resistant Jettons for I»proved Strength and Abrasion Resistance," American Dvestuff Reporter,
(November 3, 1958), pp. 758-64.
"Sales Spurt Puts New Zip Into Fabric Softeners," Chemical Week, (July 30, 1955), pp. 36-7.
"Soft Touch is Tough to Sell," Comical Week, (December 30, 1955), pp. 61-2.
Taube, R. Katherine, Enid S. Ross and Nada D. Poole. "Use of Modern Home Laundry Equipment I. "Wrinkling Effects on Swatches of Present-Dey Fabrics," American Dyestuff Reporter, (June 26, 1961), pp. 29-40.
rVard, Harold L. "Textile Softeners for Home Laundering," Journal of Home Economics, (February, 1957), pp. 122-3.
Young, Sanford P. "A Millman's Guide to Wash-Wear Finishes," Modern Textiles Magazine, (October, 1961), pp. 30-2, 57-8.
C. UNPUBLISHED MATERIAL
Armour Bthoxylated Chemicals. (Armour Industrial Chemical Company, n.d.), pp. 1-25.
Arquad 2HT Fabric Softener and Conditioner. (Armour Chemical Company, 196077 PP. 1-12.
"Home Laundry Fabric Softeners," New Yorki Jane Ashley Home Service
Department Corn Products Company, (October, 1957), pp. 1-2. Technical Data Bulletin. (Texize Chemical, Inc., n.d.), pp. 1-2.
COMPUTER PROGRAMS FOR THE STATISTICAL ANALYSIS OF DATA
I. Computer program for the statistical analysis of data for dimensional change, tear resistance, wrinkle recovery and stiffness.
N 0010 Y 0040 Z 0070 S 0070 VT 000 0062 NBBLY R276 Yl Y30 INPUT
0001 TYO T(62.) 4,N1,1,1,15, 0070 N2:-1+2XN1 ZNliYN2+Y(N2+l) 0004 Z(Hl+15)«ZNL/2 . 5,N1,31,1,36, 0069 N2:-30+Nl 0005 ZNliYN2+Y(N2+6)+Y(N2+12)+Y(N2+18)+Y(N2+24) 6,Nl,37,1,39, 0068 N2»-36+Nl 0006 ZNl:ZN2+Z(N2+3)+Z(N2+6)+Z(N2+9)+Z(N2+12) 7,N1,40,1,42, 0067 N2J-24+N1 0007 ZNliZH2+Z(N2+3)+Z(N2+6)+Z(»2+9)+Z(H2+12) 8,N1,43,1,47, 0066 N2t-128+3XN1 ZN1tZN2+Z(N2+l)+Z(N2+2) 0008 Z(Nl+6)«ZNl/6. TH F F F P F F F F F F F F F F F F F
AFP2NDIX A (Continued) 56 Z48iZ37+Z38+Z39 F 12,N1,1,1,15, F 0060 TZN1 TZ(N1+15) TZ(:Jl+30) TZ(Nl+42) F 0012 T(0) F Z54iZ48XZ48/30. F Z55«(Z37XZ37)+(Z38xZ38)+(Z39xZ39) F Z55i(Z55/lO.)-Z54 F Z56»(Z43XZ43)+(Z45XZ45)+ Z56:(Z43XZ43)+(Z44XZ44)+(Z45XZ45)+(Z46XZ46)+(Z47XZ47) F Z56«(Z56/6.)-Z54 F ZOiO. F 9,N1,1,1,15, F 0009 ZOiZO+(ZNlXZNl) F Z57:(Z0/2.)-(Z54+Z55+Z56) F Z0:0. F 10,HI,1,1,30, F 0010 Z0:Z0+(raiXYlIl) F Z58:Z0-(Z54+Z55+Z56+Z57) F Z59JZ55/2. F Z60:Z56/4. F F Z61:Z57/8 Z62:Z58/l5. Z63JZ59/Z62. Z64«Z60/Z62. Z65»Z6l/Z62. 11,Nl,54,1,58, F
APPENDIX A (Continued) 0011 TZN1 TZ(Nl+5) TZ(Nl+9) T(O.3 13,K1,57,1,58, 0013 ZNliO. G62 F F F F FF